Formation of thin
lm composite nano
ltration membrane: Effect of polysulfone
, W.J. Laua,b
, A.F. Ismaila,b,
, T. Matsuuraa,c
Advanced Membrane Technology Research Centre (AMTEC), Universiti Teknologi Malaysia, 81310 Skudai, Johor, Malaysia
bFaculty of Petroleum and Renewable Energy Engineering, Universiti Teknologi Malaysia, 81310 Skudai, Johor, Malaysia c
Department of Chemical and Biological Engineering, Industrial Membrane Research Institute, University of Ottawa, 161 Louis Pasteur St., Ottawa, ON KIN 6N5, Canada
H I G H L I G H T S
•Properties of PSf substrate membranes were fundamentally investigated. •Pore size and porosity of substrate
por-tray major role in the changes of PA layer. •TFC NF membrane made of PSf 15 wt.% substrate produced the best performance.
G R A P H I C A L A B S T R A C T
a b s t r a c t
a r t i c l e i n f o
Received 19 July 2013
Received in revised form 23 August 2013 Accepted 24 August 2013
Available online 23 September 2013
Thinﬁlm composite membrane Substrate
Polysulfone Waterﬂux Salt rejection
In this work, polysulfone (PSf) substrates with different properties were made by varying the polymer con-centration in the dope solution in the range 12–20 wt.%. Polyamide (PA) thin layers were then formed via interfacial polymerization between piperazine and trimethylchloride over the PSf substrates. Both top PA thin layers and bottom PSf substrates were characterized with respect to physicochemical properties, structural morphology, and waterﬂux/salt rejection to investigate the inﬂuence of substrate properties on the characteristics of PA thin layers. Physical properties of the PA layers were reported to be altered using different PSf substrate properties and were in good agreement with the change in water ﬂux. From the FESEM pictures, it is found that the thickness of PA layer increased as the surface pore size of sup-port membrane decreased. The change in the membrane structural properties in particular pore size is found to portray signiﬁcant contribution to the changes of formed PA layer. Interestingly, only slight changes on Na2SO4and MgSO4salt rejection were reported on any TFC membranes. Considering both
water permeability and salt rejection rate, the best performing TFC membrane produced in this work was the membrane made over substrate of 15 wt.% PSf concentration.
© 2013 Elsevier B.V. All rights reserved.
Since theﬁrst introduction in the early 1980s, nanoﬁltration (NF) membranes have attracted considerable industrial interest as a promising cost-effective material to the growing needs of separation and puriﬁ ca-tion technologies. Considering that a NF membrane has a microporous
⁎ Corresponding author at: Faculty of Petroleum and Renewable Energy Engineering, Universiti Teknologi Malaysia, 81310 Skudai, Johor, Malaysia. Tel.: +60 7 553 5592; fax: +60 7 558 1463.
E-mail addresses:firstname.lastname@example.org,email@example.com(A.F. Ismail). 0011-9164/$–see front matter © 2013 Elsevier B.V. All rights reserved.
Contents lists available atScienceDirect
pore diameter (dp) less than 2 nm, it is able to separate divalent and some
monovalent ions, dissolved organic solutes (molecular weight Mw
be-tween 200 and 500 g/mol), hardness and heavy metals, effectively[1,2]. To date, thinﬁlm composite (TFC) membrane by far is the most commer-cially successful membrane for various industrial separation processes, particularly in the water treatment and puriﬁcation applications[3–7]. The TFC membrane consists of an ultra-thin selective layer which is interfacially polymerized over a microporous substrate. The main ad-vantage of TFC membranes over asymmetric membranes is that each layer can be independently optimized to attain desired permeability and selectivity.
Up to now, various parametric studies have been conducted in an attempt to develop high performance TFC membranes by optimizing mainly the top thin selective layer. Physical and chemical properties of the substrate, however, are paid less attention during TFC mem-brane fabrication, probably because the substrate plays no signiﬁ -cant role in the solute separation and fouling reduction as the top selective layer does. The impact of substrate properties of the composite membrane formation is, therefore, less reported in the open literature during the preparation of TFC membranes. In view of the importance of a substrate to the formation of a composite membrane, several studies have been done in the past recent years to investigate the correlation between substrates made of different properties and the properties of ultrathin polyamide (PA) selective layer[10–12]. It is believed that the morphology (i.e. structure, thickness and surface charge) and the performance (i.e. permeability and selectivity) of a TFC membrane may be altered with the use of dif-ferent substrate properties[6,12,13].
In 2006, Singh et al.revealed that the change in pore size distri-bution of the polysulfone (PSf) substrate could affect the formation of a reverse osmosis TFC membrane and its performance as well. Smaller pores of PSf substrates (b70 nm) exhibited a tremendous salt rejection efﬁciency to that of bigger pores (N150 nm). This is mainly due to a no-table increase in effective layer thickness caused by the smaller pores which restrict the penetration of PA into those pores. Years later, another extensive study was also conducted by Ghosh and Hoekto investi-gate the impact of PSf support properties on the formation of composite membranes. It explained that the variance in the physical structure and chemistry of a PSf substrate apparently produced a PA with different char-acteristics and performance.
In particular, the polymer concentration in the substrate casting solution is believed to be one of the primary factors inﬂuencing the physical characteristics of the substrate. Moreover, the polymer concen-trations in the casting solution are found to be above 12 and below 20 wt.%, and mostly in the range of 15 to 18 wt.%[6,12,14–17]. There-fore, it is our intention to investigate the relationship between the phys-ical properties of substrate (i.e. surface pore size, pore size distribution and surface porosity), made of different polymer concentrations (in the range of 12–20 wt.%), and the characteristic of NF composite membrane. It is generally known that each substrate possesses its own characteristics. Therefore, the support layer itself has to form a good agreement between pore size and highﬂux to diminish the addi-tional resistance for water transport. However, to what extent would the pore structure eventually inﬂuence the composite membrane fabri-cation still remains unclear. In order to gain further insights and to achieve the objective of the present study, topographical images of each substrate surface will be further recorded by SEM and AFM follow-ing quantitative measurements described by previous studies. Thus, the obtained values from both characterizations will be discussed in detail. It should be noted that optimized conditions of PA layers, including monomer concentration, reaction time, curing temperature and time, or the addition of additives, during the TFC membrane preparation is not conducted in this study. It is expected that theﬁndings from this work would provide more insight in TFC membrane fabrication which can be generally optimized through the top PA active layer and bottom substrate layer.
Polysulfone (Udel® P-1700) purchased from Solvay Specialty Poly-mers, USA was used to fabricate substrate for TFC membrane. PSf (in pellet form) was ﬁrst dried at 100 °C overnight prior to use. Polyvinylpyrrolidone (PVP) K30 of Mw40,000 used as a pore forming
agent during substrate fabrication was purchased from Fluka Chemie GmbH, Switzerland. Trimethylchloride (TMC) and piperazine (PIP) were purchased from Sigma-Aldrich and Merck, respectively and were used to establish the PA layer on PSf substrate. 1-Methyl-2pyrrolidone (purityN99.5%) and n-Hexane supplied from Merck were used without further puriﬁcation. Na2SO4 and MgSO4 supplied by GCE Laboratory
Chemicals were used to prepare aqueous salt solution for membrane
ﬂux and rejection determination.
2.2. Membrane preparation
2.2.1. Preparation of PSf substrate
Asymmetric PSf substrates were prepared via phase inversion tech-nique using the dope formulations as shown inTable 1. In order to in-crease the porosity of PSf substrates, 1 wt.% PVP was added into dope solution and acted as a pore forming agent. To prepare the dope solu-tion, PVP wasﬁrst dissolved in NMP solvent followed by PSf. The dope solution was stirred continuously until a homogeneous polymer solu-tion was obtained. The substrate was then cast on a glass plate using the dope solution prepared. The cast substrate was kept for 30 s at am-bient temperature before immersing into a water coagulation bath at room temperature. Obtained microporous PSf support was washed thoroughly with de-ionized water to remove residual solvent followed by keeping wet at 5 °C prior to use. The substrates prepared were de-noted as PSf 12, PSf 15, PSf 18 and PSf 20, respectively, where the num-ber corresponded to the PSf concentration used in the dope solution.
2.2.2. Preparation of thin-ﬁlm composite (TFC) NF membrane
TFC NF membranes were prepared via in-situ interfacial polymeriza-tion process between PIP and TMC as shown inScheme 1. PSf substrate was initially taped onto the glass plate followed by 120 s of immersion in an aqueous solution of 2% (w/v) PIP. The excess solution from the im-pregnated membrane surface was eliminated using a soft rubber roller. The membrane was then immediately immersed into then-hexane so-lution of 0.2% (w/v) TMC for 60 s, which resulted in in-situ formation of an ultra-thin PA layer over the microporous PSf substrate. Subsequently, the resulting membrane was cured at 60 °C for 5 min andﬁnally was thoroughly washed with ionized water before storage in de-ionized water at 5 °C prior to use. The composite NF membranes pre-pared were then denoted as TFC 12, TFC 15, TFC 18 and TFC 20, respec-tively, where the number corresponded to the PSf concentration used in preparing the substrate.
2.2.3. TFC NF membrane performance evaluation
Theﬂux and rejection of fabricated TFC NF membranes were ana-lyzed using a dead-endﬁltration system (Sterlitech™HP4750 Stirred Cell) under a nitrogen atmosphere. TFC membranes were initially compacted at a trans-membrane pressure of 0.8 MPa with DI water
Dope formulation used to prepare different types of substrates. Substrate Dope formulation (wt.%)
PSf PVP NMP
PSf 12 12 1 87
PSf 15 15 1 84
PSf 18 18 1 81
for about 1 h. The active membrane surface area was 14.6 cm2. The
NF experiments were then performed using 1000 ppm Na2SO4 (or
MgSO4) solution at operating pressure and temperature set at 0.5 MPa
and 25 °C, respectively. Membrane waterﬂux (F) was subsequently measured using the following equation:
whereVis the permeate volume (L),Ais the membrane area (m2) andt
is the experimental time to obtainV(h).
A bench conductivity meter (Jenway 4520) was used to measure the salt concentration in the feed and permeate solutions. The membrane salt rejection was then determined using the following equation:
R %ð Þ ¼ 1−Cp Cf !
where,Cp is the permeate concentration (ppm) and Cf is the feed concentration (ppm), respectively.
2.3. Substrate and PA layer characterization
The chemical structure of membranes prepared was character-ized using an FTIR spectrometers FTLA2000 (ABB, Switzerland) equipped with an attenuated total reﬂection (ATR) supplied by the PIKE MIRacle™(USA). A total of 128 scans were measured during IR studies for each sample. The apparatus resolution was 8 cm−1.
The water contact angle (CA) was measured using a Phoenix 300 contact angle analyzer (S.E.O. Co., Ltd, Korea). Ten drops of de-ionized water were measured for each sample at room temperature. The aver-age of measured contact angle was reported as the CA value of the membranes. The surface roughness corrected solid–liquid interfacial free energy,−ΔGSL, was estimated using a method as described in a
previous study. The−ΔGSLcan be estimated using the following
−ΔGSL¼ γL 1þcosΔθ
where,θis the average contact angle value,Δis the relative surface area andγL= 72.8 mJ/m2(for pure water at 25 °C) is the liquid surface
ten-sion, respectively. For a smooth surface, the maximal solid–liquid inter-facial free energy is 2γLas contact angle is 0°. Subsequently, the higher
value of−ΔGSLindicates an increased hydrophilicity of the surface.
The top surface and cross-sectional morphologies of composite membranes were visualized usingﬁeld emission scanning electron mi-croscope (FESEM) (JEOL JSM-6700F). The samples were fractured in liquid nitrogen and dried under vacuum. Subsequently, membranes were sputter-coated with gold to prevent charging. Additionally, mean pore size (dpavg) and surface porosity (ε) of PSf substrates made of
dif-ferent polymer concentrations were evaluated using ImageJ software developed by the National Institute of Health (NIH) on the membrane SEM surface images. The FESEM surface images were binarized at a cer-tain threshold in order to obcer-tain a clear image of membrane surface pores following a procedure described in previous studies[19–21].
Atomic force microscopy (AFM) (Multimode 8 AFM instrument equipped with a NanoScope V controller) was used to characterize the surface morphology of the membranes in terms of mean roughness pa-rameter and pore sizes (i.e. mean pore size, geometric standard devia-tion and pore size distribudevia-tion). The scanning area of each membrane was 5μm × 5μm. The pore sizes and the probability density function curves of the substrates were determined using a previous method de-scribed by several authors[22–24].
3. Results and discussion
3.1. Effect of polymer concentration on PSf substrate properties
3.1.1. Organic functional groups
The chemical property of substrates was analyzed using an ATR-IR spectroscopy.Fig. 1shows the IR spectra of the four PSf substrates pre-pared. IR bands at 1323 cm−1, 1292 cm−1, 1242 cm−1and 1149 cm−1
were the typical characteristic peaks of the substrate made of PSf. A broad transmittance band at 1670 cm−1which corresponded to C O
stretching could indicate the presence of PVP additive in the substrate matrix. The remaining PVP entrapped in substrate also revealed that the polymeric additive had not completely leached out during phase in-version and would therefore play a role in improving substrate hydro-philicity. Overall, the chemical property of all substrates remained the same irrespective of polymer concentration used.
3.1.2. Surface morphology (FESEM)
Fig. 2presents the FESEM image of top surface of each PSf substrate made. It is seen that the pores of PSf 12, PSf 15 and PSf 18 substrates were evenly distributed throughout the substrate surface and could be easily observed when examined at a magniﬁcation of 5000×. Due to the decrease in pore size on PSf 20 substrate, these pores were unable
NH N H O Cl Cl O O Cl N N O OH O * O * n Cl H TMC PIP
Scheme 1.Interfacial polymerization of poly(piperaizine-amide).
4000 3200 2000 1600 1200 800
PSf 20 PSf 18 PSf 15
Wavenumber (cm-1) PSf 12
to be seen at the same magniﬁcation. To evaluate the effect of polymer concentration on the substrates' average pore diameter (dpavg) and
po-rosity (ε), Image J software was employed. A speciﬁc area of the surface on gray-scale SEM image was selected to convert to a black and white image which the black small spots represented the pores on the sub-strate surface. The average pore diameter values were then computed and the data are tabulated inTable 2. As expected, the pore size of sub-strate decreased with increasing polymer concentration. The decrease in pore diameter of PSf 12 substrate from 84 nm tob12 nm in PSf 20 substrate could be explained by the delayed solvent (NMP) and non-solvent (water from the coagulation bath) exchange rate during the phase inversion process which resulted from higher viscosity of dope solution used. In addition to the pore size change, it is also reported that substrate surface porosity was altered with the use of different polymer concentrations. The computed surface porosity decreased according to PSf 12 (23.04%)NPSf 15 (11.97%)NPSf 20 (10.06%)NPSf 18 (5.78%). For the PSf 12, PSf 15 and PSf 18 substrates, the results shown were in a good agreement with a previously reported study where the % surface porosity was inversely proportional with the surface pore size of substrate. It is noted that PSf 20 displayed higher surface
porosity than that of PSf 18 and this may be an error which could be caused by pores covered (resulted in size diminution) by coating element during sputter-coating process.
3.1.3. Surface roughness (AFM)
Fig. 3shows the AFM topographic images together with roughness values of PSf substrates made of different polymer concentrations. As can be seen, the surface roughness of PSf substrate was reduced with an increase in polymer concentration, indicating smaller surface pore sizes tended to create a smoother surface on a PSf substrate. The corre-lations between surface roughness and membrane pore structure have also been previously reported[22,24,25]. Using the AFM image analysis program, the pore dimension of all PSf substrates was quantitatively de-termined based on a scanning surface area of 2μm × 2μm. The mean pore sizesμpand the geometric standard deviationsσpof the substrates
as shown inTable 2were determined using a previously stated proce-dure[22–24]. The probability density function curve of each PSf sub-strate made is also presented inFig. 4in which the curves were clearly seen to be shifted to the left with increasing polymer concentration, in-dicating the decrease in substrate pore size. Comparisons made be-tween the pore size obtained from AFM images and FESEM images showed the same decreasing pore size trend (with increasing polymer concentration), but the pore size determined from the AFM image was bigger. This is mainly because of the diminution of pore sizes due to a coating procedure that is generally required for FESEM characterization [24,26].
3.1.4. Waterﬂux and surface hydrophilicity
With respect to waterﬂux and surface hydrophilicity, it is also found that both properties were inﬂuenced by the polymer concentration used in preparing substrates.Table 3shows effect of PSf concentration
Fig. 2.FESEM images of top surface of PSf substrates, a) PSf 12, (b) PSf 15, (c) PSf 18 and (d) PSf 20. (Note: threshold image placed on the bottom left corner of each SEM image was used to determine the average pore size and porosity of PSf substrate).
The mean pore size (μp), geometric standard deviation (σp), average pore diameter (dpavg)
and surface porosity (ε) of PSf substrates prepared from different polymer concentrations. Substrate AFM measurement SEM measurement
μp(nm) σp(nm) dpavg(nm) ε(%)
on the substrate properties with respect to pure water permeability, contact angle and the surface area corrected interfacial free energy (−ΔGSL). Owing to the decrease in substrate pore size as discussed
in the previous section (Section 3.1.2), the decrease in waterﬂux of
PSf 20 substrate to 20.3 from 683.1 L/m2·h·bar reported in PSf 12
sub-strate was reasonable and followed the trend of change. The water con-tact angle on the other hand was found to increase slightly from 66.3° to 70.8° with increasing PSf concentration from 12 to 20 wt.%. The small increase in contact angle value could not be used to show the increased hydrophobicity of substrate as the substrate surface roughness might also contribute to the change of contact angle value[18,27]. Therefore, instead of contact angle value,−ΔGSLwas considered as a better
deter-mination of surface hydrophilicity. Results showed that the degree of surface hydrophilicity reduced (lower−ΔGSLvalue) with increasing
polymer concentration, revealing that theﬂux reduction in substrate could also be due to the decrease in surface hydrophilicity in addition to pore dimension and surface roughness.
Based on the characterization on the substrate properties, it is hy-pothesized that the properties of TFC membranes could be altered
Fig. 3.3D AFM images of PSf substrates together with surface roughness values, (a) PSf 12, (b) PSf 15, (c) PSf 18 and (d) PSf 20.
0 30 60 90 120 150 180
0.00 0.01 0.02 0.03 0.04
Probability density function,
Pore size (nm)
PSf12 PSf15 PSf18 PSf20
Fig. 4.Probability density function curves of different PSf substrates.
Properties of substrates with respect to pure water permeability, contact angle and−ΔGSL.
Substrate Pure water permeability (L/m2
Contact angle (°) −ΔGSL
using PSf substrates of different properties (e.g. pore size, surface poros-ity, surface roughness and hydrophilicity). In the following section, we will investigate to what extent the changes in substrate properties
would affect the characteristics of PA layer formation and further the performance of TFC NF membrane during theﬁltration process.
3.2. Effect of polymer concentration on TFC NF membrane properties
3.2.1. Organic functional groups of PA layer
Fig. 5shows the IR spectra of the polyamide TFC membranes pre-pared from different substrate properties. The IR spectra indicated that the interfacial polymerization between PIP and TMC was successfully formed over all PSf substrates owing to the presence of strong band at 1620 cm−1. This peak was corresponded to the C O band of an amide
group. In addition, a broad band found at 3440 cm−1could be assigned to the presence of–COOH groups formed in PA thin layer. The appear-ance of carboxylic acid functional groups is attributed to the partial hy-drolysis of the acyl chloride unit of TMC. Overall, the IR spectra revealed that PA layer could still be established even though there was a signiﬁcant change in substrate properties, particularly the pore size of the substrate.
3.2.2. Surface roughness and morphology of PA layer
The surface roughness of TFC membranes was characterized using AFM analysis and the 3D topographic together with roughness values is presented inFig. 6. Compared to the surface roughness of PSf substrates (seeFig. 3), the signiﬁcant increase in surface roughness on composite membranes was well-matched with the typical ridge-valley structure of 4000 3200 2000 1800 1600 1400 1200 1000 800
Wavenumber (cm-1) 1620
TFC 20 TFC 18 TFC 15 TFC 12
Fig. 5.ATR-IR spectra of TFC NF membranes prepared over different PSf substrates.
PA layers. Though the roughness of PSf substrate decreased with increas-ing polymer concentration, the roughness of TFC membranes prepared showed the opposite trend in which TFC 20 membrane displayed the highest roughness value while TFC 12 membrane the lowest. In view of this, it is fair to say that substrate roughness might not be the main factor governing the changes in TFC surface roughness.
Representative FESEM top surface and cross-sectional images of TFC membranes are also presented inFigs. 7 and 8, respectively. In the im-ages of the top surface, the white parts represented the peaks while the dark areas corresponded to the valleys. The variation in the surface morphology of TFC membrane compared to the PSf substrate conﬁrmed
that PA active layer was successfully formed over PSf substrate. Clearly, there was a change in PA layer structure with the use of different substrate properties. The TFC 12 and TFC 15 membranes prepared from low polymer concentration substrates exhibited uniformly formed
“ridge-and-valley”like structure. Further increases in the polymer con-centration of substrate tended to cover the valleyﬁlm, increasing the ridge portion of PA layer as evidenced in TFC 18 membrane. This, as a consequence, resulted in the increase in PA layer thickness as evidenced on the cross-sectional image of the membrane. For TFC 20 membrane, it is believed that the nodular structures drawn as white circles inFig. 8 (d) resulted from the tight pore structure of the substrate used. The
existence of these nodular structures gave quantitatively rougher sur-face morphology and increased PA layer thickness which is consistent with the AFM analysis and FESEM analysis, respectively. It must be pointed out that the irregular morphology of PA layer would preclude precise quantiﬁcation of the layer thickness. Nevertheless, based on the cross-sectional images captured at a magniﬁcation of 25,000×, it can be seen that there was a signiﬁcant increase in PA layer thickness with increasing substrate's polymer concentration. The variation of PA layer thickness can be explained by the fact that bigger pores of sub-strate would allow the PIP aqueous solution to diffuse deep into the pore channel, leading to the possibility of PA cross-linking inside the pores. On the other hand, smaller pores would limit the diffusion of PIP aqueous solution deep into the pores, developing thicker PA layer and greater surface roughness as evidenced in the work of Singh et. al
. Yet another interpretation is on the assumption that PIP is supplied to the organic and aqueous phase interface by the diffusion through the pores of the substrate skin layer from the pool of the aqueous phase in the porous sublayer, and this is the rate controlling step for the PIP sup-ply. Unlike pressure-drivenﬁltration, the PIP supply rate should be pro-portional to the effective porosity of the substrate membrane, ε/δ, whereεandδare the porosity and thickness of the substrate skin layer, respectively. The ratio ofε/δof PSf 20 membrane to that of PSf 12 mem-brane can be easily calculated by applying the Poiseuille equation to the measured pore size and the pure water permeationﬂux of the respective membranes, and the result is 1.54. This value is close to the thickness ratio (~1.8) of PSf 20 to PSf 12 membrane. Interestingly, the decrease in the pore size results in the more quick supply of PIP to the interface, and hence the increase in the PA layer thickness, due to the decrease inδ.
3.2.3. Waterﬂux and salt rejection
Experimental data ofﬂux, salt rejections and water contact angle of TFC membranes are outlined inFig. 9. The error bars indicated the stan-dard deviations of average measured values. With respect to waterﬂux, it is reported that theﬂux decreased in the order of TFC 15NTFC 18≥TFC 12NTFC 20. These results obtained were mainly inﬂuenced by the varied morphology of PA layer formed over the different PSf sub-strates. The lowestﬂux reported in TFC 20 membrane is most likely due to the signiﬁcant increase in PA selective layer thickness, creating addi-tional resistance for water transport through the membrane. An in-crease in ridge portion as found in TFC 18 membrane could also be the reason lowering theﬂux of the prepared membrane. Though TFC 12 and TFC 15 membranes exhibited very similar“ridge-and-valley”like structure, the waterﬂux shown by each membrane was quite different. This may be explained by the formation of PA layer inside the pores as have been discussed in the previous section (Section 3.2.2), resulting in a drop in water permeation rate.
Comparing Na2SO4(with monovalent cation) rejection with MgSO4
(with divalent cation), the former is higher than the latter, indicating the presence of residual–COCl functional groups in the TMC monomer that are unreacted for cross-linking during IP process. These COCls are later hydrolyzed to COOHs in aqueous solution which give negative charge to the membrane, causing the rejection of Na2SO4higher than
MgSO4. Overall, based on the AFM and FESEM analysis, we are
con-vinced that the physical characteristics of PA layer e.g. layer thickness and surface roughness could be obviously altered using different sub-strate properties which, as a result, affected the water permeation rate. It must be emphasized that theﬁndings obtained in this study might differ if the substrate is made of another type of polymer and/or with the presence of other additives. Thus, the results shown here were based on the observations on substrates made of commonly used PSf with the mean pore size in the range 38–86 nm (based on AFM analysis), water contact angle between 66 and 70°, Ravalue of
6.5–14 nm and waterﬂux of 20–680 L/m2·h·bar.
The correlation between the poly(piperazine-amide) layer and the underlying PSf substrate was fundamentally investigated on TFC NF membranes. PSf substrates with different properties were prepared by
varying the concentration of polymer in the dope solution ranging from 12 to 20 wt.%. Among the parameters investigated, it is found that pore size and surface porosity of PSf substrates were obviously al-tered with increasing polymer concentration in which higher concen-tration of polymer tended to produce smaller pore size and lower surface porosity, leading to reduction in pure water permeability. Re-sults from ATR-IR spectra revealed that the speciﬁc functional group of PA was able to be detected over all PSf substrates regardless of the prop-erties, conﬁrming the successful formation of TFC membrane. Based on the AFM and FESEM analyses, it is reported that the physical properties of PA layer were changed using different PSf substrate properties, which were consistent with the change in waterﬂux. Based on the FESEM pic-tures, it is found that the thickness of PA layer increased as the pores size decreased. The change in the membrane structural properties in partic-ular pore size is found to portray signiﬁcant contribution to the changes of formed PA layer. It was further postulated that PIP is supplied to the organic and aqueous phase interface by diffusion through the pores at the substrate skin layer from the pool of aqueous phase in the porous sublayer, and this is the rate controlling step for the PIP supply. Addi-tionally, it was found that substrate roughness might not be the main factor governing the changes in TFC surface roughness. Overall, it is cluded that the TFC membrane made over substrate of 15 wt.% PSf con-centration with an average pore size of 47.20 nm and 11.97% of surface porosity (SEM measurement) was the optimum membrane by taking into account both water permeability and salt rejection. Theﬁndings shown in this work have provided an answer as to why a PSf substrate made of 15 wt.% polymer concentration was widely employed as supporting membrane for TFC membrane fabrication, whether in the past or present.
The authors are grateful for the researchﬁnancial support by the Ministry of Higher Education under Long-term Research Grant Scheme (Vot no. 4L803) and Universiti Teknologi Malaysia under Research University Grant Scheme (Vot no. Q.J.130000.7142.01H40). Author, N. Misdan thanks the sponsorship given by Ministry of Higher Education under MyBrain15 (MyPhD) scheme during her Ph.D. studies. The authors also gratefully thank Prof. Y. M. Lee in the WCU Department of Energy Engineering at Hanyang University (South Korea) for providing some in-struments for the membrane characterization. Authors are also very grateful to Mr. D. W. Shin for performing the AFM characterizations.
 M. Ulbricht, Advanced functional polymer membranes, Polymer 47 (2006) 2217–
 J. Cadotte, R. Forester, M. Kim, R. Petersen, T. Stocker, Nanoﬁltration membranes broaden the use of membrane separation technology, Desalination 70 (1988) 77–88.
 A. Rahimpour, M. Jahanshahi, N. Mortazavian, S.S. Madaeni, Y. Mansourpanah, Prep-aration and characterization of asymmetric polyethersulfone and thin-ﬁlm compos-ite polyamide nanoﬁltration membranes for water softening, Appl. Surf. Sci. 256 (2010) 1657–1663.
 R.S. Harisha, K.M. Hosamani, R.S. Keri, S.K. Nataraj, T.M. Aminabhavi, Arsenic removal from drinking water using thinﬁlm composite nanoﬁltration membrane, Desalination 252 (2010) 75–80.
 W.-J. Lau, A.F. Ismail, Polymeric nanoﬁltration membranes for textile dye wastewater treatment: preparation, performance evaluation, transport modelling, and fouling control—a review, Desalination 245 (2009) 321–348.
 L. Hu, S. Zhang, R. Han, X. Jian, Preparation and performance of novel thermally stable polyamide/PPENK composite nanoﬁltration membranes, Appl. Surf. Sci. 258 (2012) 9047–9053.
 A.F. Ismail, W.J. Lau, Inﬂuence of feed conditions on the rejection of salt and dye in aqueous solution by different characteristics of hollowﬁber nanoﬁltration mem-branes, Desalin. Water Treat. 6 (2009) 281–288.
 R.J. Petersen, Composite reverse osmosis and nanoﬁltration membranes, J. Membr. Sci. 83 (1993) 81–150.
 W.J. Lau, A.F. Ismail, N. Misdan, M.A. Kassim, A recent progress in thinﬁlm compos-ite membrane: a review, Desalination 287 (2012) 190–199.
 P.S. Singh, S.V. Joshi, J.J. Trivedi, C.V. Devmurari, A.P. Rao, P.K. Ghosh, Probing the structural variations of thinﬁlm composite RO membranes obtained by coating
TFC 12 TFC 15 TFC 18 TFC 20 0 10 20 30 40 50 60 70 80 90 100 Relative Values Flux (LMH)
MgSO4 Rejection (%) Na2SO4 Rejection (%) Contact angle (0)
polyamide over polysulfone membranes of different pore dimensions, J. Membr. Sci. 278 (2006) 19–25.
 H.I. Kim, S.S. Kim, Plasma treatment of polypropylene and polysulfone supports for thinﬁlm composite reverse osmosis membrane, J. Membr. Sci. 286 (2006) 193–201.
 A.K. Ghosh, E.M.V. Hoek, Impacts of support membrane structure and chemistry on polyamide–polysulfone interfacial composite membranes, J. Membr. Sci. 336 (2009) 140–148.
 G.Z. Ramon, M.C.Y. Wong, E.M.V. Hoek, Transport through composite membrane, part 1: is there an optimal support membrane? J. Membr. Sci. 415–416 (2012) 298–305.
 A. Prakash Rao, N.V. Desai, R. Rangarajan, Interfacially synthesized thin ﬁlm composite RO membranes for seawater desalination, J. Membr. Sci. 124 (1997) 263–272.
 N.K. Saha, S.V. Joshi, Performance evaluation of thinﬁlm composite polyamide nanoﬁltration membrane with variation in monomer type, J. Membr. Sci. 342 (2009) 60–69.
 A. Soroush, J. Barzin, M. Barikani, M. Fathizadeh, Interfacially polymerized polyamide thinﬁlm composite membranes: preparation, characterization and performance evaluation, Desalination 287 (2012) 310–316.
 A.L. Ahmad, B.S. Ooi, Properties–performance of thinﬁlm composites membrane: study on trimesoyl chloride content and polymerization time, J. Membr. Sci. 255 (2005) 67–77.
 A.K. Ghosh, B.-H. Jeong, X. Huang, E.M.V. Hoek, Impacts of reaction and curing conditions on polyamide composite reverse osmosis membrane properties, J. Membr. Sci. 311 (2008) 34–45.
 I. Masselin, L. Durand-Bourlier, J.-M. Laine, P.-Y. Sizaret, X. Chasseray, D. Lemordant, Membrane characterization using microscopic image analysis, J. Membr. Sci. 186 (2001) 85–96.
 S. Zhao, Z. Wang, X. Wei, B. Zhao, J. Wang, S. Yang, S. Wang, Performance improve-ment of polysulfone ultraﬁltration membrane using PANiEB as both pore forming agent and hydrophilic modiﬁer, J. Membr. Sci. 385–386 (2011) 251–262.
 G.R. Guillen, T.P. Farrell, R.B. Kaner, E.M.V. Hoek, Pore-structure, hydrophilicity, and particleﬁltration characteristics of polyaniline–polysulfone ultraﬁltration mem-branes, J. Mater. Chem. 20 (2010) 4621–4628.
 M. Khayet, C.Y. Feng, K.C. Khulbe, T. Matsuura, Preparation and characterization of polyvinylideneﬂuoride hollow ﬁber membranes for ultraﬁltration, Polymer 43 (2002) 3879–3890.
 M.C. García-Payo, M. Essalhi, M. Khayet, Effects of PVDF-HFP concentration on mem-brane distillation performance and structural morphology of hollowﬁber membranes, J. Membr. Sci. 347 (2010) 209–219.
 S. Singh, K.C. Khulbe, T. Matsuura, P. Ramamurthy, Membrane characterization by solute transport and atomic force microscopy, J. Membr. Sci. 142 (1998) 111–127.
 A. Bessières, M. Meireles, R. Coratger, J. Beauvillain, V. Sanchez, Investigations of sur-face properties of polymeric membranes by nearﬁeld microscopy, J. Membr. Sci. 109 (1996) 271–284.
 A.K. Fritzsche, A.R. Arevalo, A.F. Connolly, M.D. Moore, V. Elings, C.M. Wu, The struc-ture and morphology of the skin of polyethersulfone ultraﬁltration membranes: a comparative atomic force microscope and scanning electron microscope study, J. Appl. Polym. Sci. 45 (1992) 1945–1956.
 M. Fathizadeh, A. Aroujalian, A. Raisi, Effect of lag time in interfacial polymerization on polyamide composite membrane with different hydrophilic sub layers, Desalination 284 (2012) 32–41.